LMucko/crystallography-open-database huggingface dataset:
Temperature dependence of the cation distribution in nickel aluminate (NiAl2O4) spinel: a powder XRD study Sample: quenched from 1200 C, held for 10m, Bayerisheches Geoinstitut (Mo), Model 2
O'Neill H St C; Dollase, W. A.; Ross, C. R.; Physics and Chemistry of Minerals 18 (1991) 302–319; doi:

data_9005988
_publ_section_title
;Temperature dependence of the cation distribution in nickel aluminate
 (NiAl2O4) spinel: a powder XRD study Sample: quenched from 1200 C, held for
 10m, Bayerisheches Geoinstitut (Mo), Model 2
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              302
_journal_page_last               319
_journal_volume                  18
_journal_year                    1991
_chemical_formula_structural     NiAl2O4
_chemical_formula_sum            'Al2 Ni O4'
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.0517
_cell_length_b                   8.0517
_cell_length_c                   8.0517
_cell_volume                     521.991
_database_code_amcsd             0007570
_exptl_crystal_density_diffrn    4.496
_exptl_crystal_thermal_history   'quenched from 1200 C, held for 10m'
_cod_duplicate_entry             9005963
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Ni Al2) O4'
_cod_database_code               9005988
Temperature dependence of the cation distribution in nickel aluminate (NiAl2O4) spinel: a powder XRD study Sample: quenched from 1250 C, held for 10m, Bayerisheches Geoinstitut (Mo), Model 2
O'Neill H St C; Dollase, W. A.; Ross, C. R.; Physics and Chemistry of Minerals 18 (1991) 302–319; doi:

data_9005989
_publ_section_title
;Temperature dependence of the cation distribution in nickel aluminate
 (NiAl2O4) spinel: a powder XRD study Sample: quenched from 1250 C, held for
 10m, Bayerisheches Geoinstitut (Mo), Model 2
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              302
_journal_page_last               319
_journal_volume                  18
_journal_year                    1991
_chemical_formula_structural     NiAl2O4
_chemical_formula_sum            'Al2 Ni O4'
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.0452
_cell_length_b                   8.0452
_cell_length_c                   8.0452
_cell_volume                     520.728
_database_code_amcsd             0007571
_exptl_crystal_density_diffrn    4.507
_exptl_crystal_thermal_history   'quenched from 1250 C, held for 10m'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Ni Al2) O4'
_cod_database_code               9005989
Temperature dependence of the cation distribution in nickel aluminate (NiAl2O4) spinel: a powder XRD study Sample: quenched from 700 C, held for 43d, UCLA (Cu), Model 2
O'Neill H St C; Dollase, W. A.; Ross, C. R.; Physics and Chemistry of Minerals 18 (1991) 302–319; doi:

data_9005990
_publ_section_title
;
 Temperature dependence of the cation distribution in nickel
 aluminate (NiAl2O4) spinel: a powder XRD study
 Sample: quenched from 700 C, held for 43d, UCLA (Cu), Model 2
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              302
_journal_page_last               319
_journal_volume                  18
_journal_year                    1991
_chemical_formula_structural     NiAl2O4
_chemical_formula_sum            'Al2 Ni O4'
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.0452
_cell_length_b                   8.0452
_cell_length_c                   8.0452
_cell_volume                     520.728
_database_code_amcsd             0007572
_exptl_crystal_density_diffrn    4.507
_exptl_crystal_thermal_history   'quenched from 700 C, held for 43d'
_cod_duplicate_entry             9005965
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Ni Al2) O4'
_cod_database_code               9005990
Temperature dependence of the cation distribution in nickel aluminate (NiAl2O4) spinel: a powder XRD study Sample: quenched from 750 C, held for 80h, UCLA (Cu), Model 2
O'Neill H St C; Dollase, W. A.; Ross, C. R.; Physics and Chemistry of Minerals 18 (1991) 302–319; doi:

data_9005991
_publ_section_title
;
 Temperature dependence of the cation distribution in nickel
 aluminate (NiAl2O4) spinel: a powder XRD study
 Sample: quenched from 750 C, held for 80h, UCLA (Cu), Model 2
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              302
_journal_page_last               319
_journal_volume                  18
_journal_year                    1991
_chemical_formula_structural     NiAl2O4
_chemical_formula_sum            'Al2 Ni O4'
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.0460
_cell_length_b                   8.0460
_cell_length_c                   8.0460
_cell_volume                     520.883
_database_code_amcsd             0007573
_exptl_crystal_density_diffrn    4.505
_exptl_crystal_thermal_history   'quenched from 750 C, held for 80h'
_cod_duplicate_entry             9005966
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Ni Al2) O4'
_cod_database_code               9005991
Temperature dependence of the cation distribution in nickel aluminate (NiAl2O4) spinel: a powder XRD study Sample: quenched from 750 C, held for 43h, UCLA (Cu), Model 2
O'Neill H St C; Dollase, W. A.; Ross, C. R.; Physics and Chemistry of Minerals 18 (1991) 302–319; doi:

data_9005992
_publ_section_title
;
 Temperature dependence of the cation distribution in nickel
 aluminate (NiAl2O4) spinel: a powder XRD study
 Sample: quenched from 750 C, held for 43h, UCLA (Cu), Model 2
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              302
_journal_page_last               319
_journal_volume                  18
_journal_year                    1991
_chemical_formula_structural     NiAl2O4
_chemical_formula_sum            'Al2 Ni O4'
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.0460
_cell_length_b                   8.0460
_cell_length_c                   8.0460
_cell_volume                     520.883
_database_code_amcsd             0007574
_exptl_crystal_density_diffrn    4.505
_exptl_crystal_thermal_history   'quenched from 750 C, held for 43h'
_cod_duplicate_entry             9005954
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Ni Al2) O4'
_cod_database_code               9005992
Temperature dependence of the cation distribution in nickel aluminate (NiAl2O4) spinel: a powder XRD study Sample: quenched from 800 C, held for 11d, UCLA (Cu), Model 2
O'Neill H St C; Dollase, W. A.; Ross, C. R.; Physics and Chemistry of Minerals 18 (1991) 302–319; doi:

data_9005993
_publ_section_title
;
 Temperature dependence of the cation distribution in nickel
 aluminate (NiAl2O4) spinel: a powder XRD study
 Sample: quenched from 800 C, held for 11d, UCLA (Cu), Model 2
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              302
_journal_page_last               319
_journal_volume                  18
_journal_year                    1991
_chemical_formula_structural     NiAl2O4
_chemical_formula_sum            'Al2 Ni O4'
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.0460
_cell_length_b                   8.0460
_cell_length_c                   8.0460
_cell_volume                     520.883
_database_code_amcsd             0007575
_exptl_crystal_density_diffrn    4.505
_exptl_crystal_thermal_history   'quenched from 800 C, held for 11d'
_cod_duplicate_entry             9005968
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Ni Al2) O4'
_cod_database_code               9005993
Temperature dependence of the cation distribution in nickel aluminate (NiAl2O4) spinel: a powder XRD study Sample: quenched from 850 C, held for 49h, UCLA (Cu), Model 2
O'Neill H St C; Dollase, W. A.; Ross, C. R.; Physics and Chemistry of Minerals 18 (1991) 302–319; doi:

data_9005994
_publ_section_title
;
 Temperature dependence of the cation distribution in nickel
 aluminate (NiAl2O4) spinel: a powder XRD study
 Sample: quenched from 850 C, held for 49h, UCLA (Cu), Model 2
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              302
_journal_page_last               319
_journal_volume                  18
_journal_year                    1991
_chemical_formula_structural     NiAl2O4
_chemical_formula_sum            'Al2 Ni O4'
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.0468
_cell_length_b                   8.0468
_cell_length_c                   8.0468
_cell_volume                     521.038
_database_code_amcsd             0007576
_exptl_crystal_density_diffrn    4.504
_exptl_crystal_thermal_history   'quenched from 850 C, held for 49h'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Ni Al2) O4'
_cod_database_code               9005994
Temperature dependence of the cation distribution in nickel aluminate (NiAl2O4) spinel: a powder XRD study Sample: quenched from 901 C, held for 16h, UCLA (Cu), Model 2
O'Neill H St C; Dollase, W. A.; Ross, C. R.; Physics and Chemistry of Minerals 18 (1991) 302–319; doi:

data_9005995
_publ_section_title
;
 Temperature dependence of the cation distribution in nickel
 aluminate (NiAl2O4) spinel: a powder XRD study
 Sample: quenched from 901 C, held for 16h, UCLA (Cu), Model 2
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              302
_journal_page_last               319
_journal_volume                  18
_journal_year                    1991
_chemical_formula_structural     NiAl2O4
_chemical_formula_sum            'Al2 Ni O4'
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.0473
_cell_length_b                   8.0473
_cell_length_c                   8.0473
_cell_volume                     521.135
_database_code_amcsd             0007577
_exptl_crystal_density_diffrn    4.503
_exptl_crystal_thermal_history   'quenched from 901 C, held for 16h'
_cod_duplicate_entry             9005970
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Ni Al2) O4'
_cod_database_code               9005995
Temperature dependence of the cation distribution in nickel aluminate (NiAl2O4) spinel: a powder XRD study Sample: quenched from 950 C, held for 16h, UCLA (Cu), Model 2
O'Neill H St C; Dollase, W. A.; Ross, C. R.; Physics and Chemistry of Minerals 18 (1991) 302–319; doi:

data_9005996
_publ_section_title
;
 Temperature dependence of the cation distribution in nickel
 aluminate (NiAl2O4) spinel: a powder XRD study
 Sample: quenched from 950 C, held for 16h, UCLA (Cu), Model 2
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              302
_journal_page_last               319
_journal_volume                  18
_journal_year                    1991
_chemical_formula_structural     NiAl2O4
_chemical_formula_sum            'Al2 Ni O4'
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.0481
_cell_length_b                   8.0481
_cell_length_c                   8.0481
_cell_volume                     521.291
_database_code_amcsd             0007578
_exptl_crystal_density_diffrn    4.502
_exptl_crystal_thermal_history   'quenched from 950 C, held for 16h'
_cod_duplicate_entry             9005958
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Ni Al2) O4'
_cod_database_code               9005996
Temperature dependence of the cation distribution in nickel aluminate (NiAl2O4) spinel: a powder XRD study Sample: quenched from 1000 C, held for 1h, UCLA (Cu), Model 2
O'Neill H St C; Dollase, W. A.; Ross, C. R.; Physics and Chemistry of Minerals 18 (1991) 302–319; doi:

data_9005997
_publ_section_title
;
 Temperature dependence of the cation distribution in nickel
 aluminate (NiAl2O4) spinel: a powder XRD study
 Sample: quenched from 1000 C, held for 1h, UCLA (Cu), Model 2
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              302
_journal_page_last               319
_journal_volume                  18
_journal_year                    1991
_chemical_formula_structural     NiAl2O4
_chemical_formula_sum            'Al2 Ni O4'
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.0488
_cell_length_b                   8.0488
_cell_length_c                   8.0488
_cell_volume                     521.427
_database_code_amcsd             0007579
_exptl_crystal_density_diffrn    4.501
_exptl_crystal_thermal_history   'quenched from 1000 C, held for 1h'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Ni Al2) O4'
_cod_database_code               9005997
Temperature dependence of the cation distribution in nickel aluminate (NiAl2O4) spinel: a powder XRD study Sample: quenched from 1050 C, held for 1h, UCLA (Cu), Model 2
O'Neill H St C; Dollase, W. A.; Ross, C. R.; Physics and Chemistry of Minerals 18 (1991) 302–319; doi:

data_9005998
_publ_section_title
;
 Temperature dependence of the cation distribution in nickel
 aluminate (NiAl2O4) spinel: a powder XRD study
 Sample: quenched from 1050 C, held for 1h, UCLA (Cu), Model 2
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              302
_journal_page_last               319
_journal_volume                  18
_journal_year                    1991
_chemical_formula_structural     NiAl2O4
_chemical_formula_sum            'Al2 Ni O4'
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.0497
_cell_length_b                   8.0497
_cell_length_c                   8.0497
_cell_volume                     521.602
_database_code_amcsd             0007580
_exptl_crystal_density_diffrn    4.499
_exptl_crystal_thermal_history   'quenched from 1050 C, held for 1h'
_cod_duplicate_entry             9005973
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Ni Al2) O4'
_cod_database_code               9005998
Temperature dependence of the cation distribution in nickel aluminate (NiAl2O4) spinel: a powder XRD study Sample: quenched from 1100 C, held for 35m, UCLA (Cu), Model 2
O'Neill H St C; Dollase, W. A.; Ross, C. R.; Physics and Chemistry of Minerals 18 (1991) 302–319; doi:

data_9005999
_publ_section_title
;
 Temperature dependence of the cation distribution in nickel
 aluminate (NiAl2O4) spinel: a powder XRD study
 Sample: quenched from 1100 C, held for 35m, UCLA (Cu), Model 2
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              302
_journal_page_last               319
_journal_volume                  18
_journal_year                    1991
_chemical_formula_structural     NiAl2O4
_chemical_formula_sum            'Al2 Ni O4'
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.0504
_cell_length_b                   8.0504
_cell_length_c                   8.0504
_cell_volume                     521.738
_database_code_amcsd             0007581
_exptl_crystal_density_diffrn    4.498
_exptl_crystal_thermal_history   'quenched from 1100 C, held for 35m'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Ni Al2) O4'
_cod_database_code               9005999
Temperature dependence of the cation distribution in nickel aluminate (NiAl2O4) spinel: a powder XRD study Sample: quenched from 1150 C, held for 5m, UCLA (Cu), Model 2
O'Neill H St C; Dollase, W. A.; Ross, C. R.; Physics and Chemistry of Minerals 18 (1991) 302–319; doi:

data_9006000
_publ_section_title
;
 Temperature dependence of the cation distribution in nickel
 aluminate (NiAl2O4) spinel: a powder XRD study
 Sample: quenched from 1150 C, held for 5m, UCLA (Cu), Model 2
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              302
_journal_page_last               319
_journal_volume                  18
_journal_year                    1991
_chemical_formula_structural     NiAl2O4
_chemical_formula_sum            'Al2 Ni O4'
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.0511
_cell_length_b                   8.0511
_cell_length_c                   8.0511
_cell_volume                     521.874
_database_code_amcsd             0007582
_exptl_crystal_density_diffrn    4.497
_exptl_crystal_thermal_history   'quenched from 1150 C, held for 5m'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Ni Al2) O4'
_cod_database_code               9006000
Temperature dependence of the cation distribution in nickel aluminate (NiAl2O4) spinel: a powder XRD study Sample: quenched from 1200 C, held for 10m, UCLA (Cu), Model 2
O'Neill H St C; Dollase, W. A.; Ross, C. R.; Physics and Chemistry of Minerals 18 (1991) 302–319; doi:

data_9006001
_publ_section_title
;
 Temperature dependence of the cation distribution in nickel
 aluminate (NiAl2O4) spinel: a powder XRD study
 Sample: quenched from 1200 C, held for 10m, UCLA (Cu), Model 2
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              302
_journal_page_last               319
_journal_volume                  18
_journal_year                    1991
_chemical_formula_structural     NiAl2O4
_chemical_formula_sum            'Al2 Ni O4'
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.0517
_cell_length_b                   8.0517
_cell_length_c                   8.0517
_cell_volume                     521.991
_database_code_amcsd             0007583
_exptl_crystal_density_diffrn    4.496
_exptl_crystal_thermal_history   'quenched from 1200 C, held for 10m'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Ni Al2) O4'
_cod_database_code               9006001
Temperature dependence of the cation distribution in nickel aluminate (NiAl2O4) spinel: a powder XRD study Sample: quenched from 1250 C, held for 10m, UCLA (Cu), Model 2
O'Neill H St C; Dollase, W. A.; Ross, C. R.; Physics and Chemistry of Minerals 18 (1991) 302–319; doi:

data_9006002
_publ_section_title
;
 Temperature dependence of the cation distribution in nickel
 aluminate (NiAl2O4) spinel: a powder XRD study
 Sample: quenched from 1250 C, held for 10m, UCLA (Cu), Model 2
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              302
_journal_page_last               319
_journal_volume                  18
_journal_year                    1991
_chemical_formula_structural     NiAl2O4
_chemical_formula_sum            'Al2 Ni O4'
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.0522
_cell_length_b                   8.0522
_cell_length_c                   8.0522
_cell_volume                     522.088
_database_code_amcsd             0007584
_exptl_crystal_density_diffrn    4.495
_exptl_crystal_thermal_history   'quenched from 1250 C, held for 10m'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Ni Al2) O4'
_cod_database_code               9006002